October 2018, Vol. 18, No. 5 MANUFACTURING TECHNOLOGY ISSN 1213–2489 Fatigue Life of Al-Honeycomb Core Composites Construction Alexander Čapka, Sona Rusnakova, Milan Žaludek, Konstantinos Karvanis Department of Production Engineering, Faculty of Technology, Tomas Bata University in Zlín. Vavrečkova 275, 760 01 Zlín. Czech Republic. E-mail: [email protected], [email protected], [email protected], [email protected] Polymer composite honeycomb sandwich panels (PCHSPs) are used in many sectors of industry, such as in aerospace, defense and public transport factory. Sandwich panels consist of two facing skins and the core. Products of all industry sectors have to meet requirements on their dependability. This research paper deals with a proposal of the most appropriate methodology for dependability testing of PCHSPs products used in transport industry. Dependability is a global concept that includes terms such as availability, reliability, durability, maintainability, supportability, etc. The experiments have shown S-N curves with damages and without damages of PCHSPs. An important part of dependability is to be fonded the limit states of the studied object, which are for PCHSPs are characterized by fiber cracking and (core) delamination. Dependability evaluation consists of analysis and tests. For every test, it is necessary to be developed its test plan. Facing skin components of the sandwich panels may particularly be damaged. There are several methods of non-destructive testing, which can be used to determine the damage of facing skins of sandwich panels. Infrared thermography (IRNDT) is one of them. IRNDT utilizes thermo-physical properties of the materials, including thermal diffusivity. Keywords: composite sandwich panel, honeycomb core, three-point bending, S-N curve, fatigue life Introduction The composite materials (CM) are increasingly replacing conventional structural and building materials. A special type of composite material is the polymer composite sandwich panel with a honeycomb core (PCHSP). PCHSPs have been used in aviation since the 1960s. First on tertiary structures, later on secondary and nowadays on primary structures. At present, PCHSPs are also used in the construction of land vehicles (cars and buses, railway trains, etc.). The design of the aircraft and land vehicles is stressed by flight and ground loads (surface loads: aerodynamic, volume loads: own weight, etc.). These are always random processes. This work deals with statistical analysis of PCHSP testing. The substance of evaluation is in the determination of PCHSP´s lifetime. The issue of fatigue loading of PCHSPs is not fully explored and general conclusions have not been formed yet. Unlike metallic materials, where two standards [1] and [2] for metal fatigue testing used in the Czech Republic, however, there is no specialized standard describing testing and statistical evaluation of PCHSP´s fatigue lifetime. There is only ISO 13003:2003 standard [3], which is applicable to composite materials (laminates) and the military standards; MIL-HDBK-23A [4]. There is a relatively small number of scientific publications dealing with the life fatigue test of PCHSPs. Only static tests on sandwich panels are included in the book [5] and fatigue tests of composite structures are described in [6] (laminates only). There is also a limited number of scientific articles dealing with PCHSPs fatigue tests [7, 8, 9, and 10]. The issue of fatigue testing of sandwich panels was solved in Czechoslovakia already in 1972 [11]. A PCHSP has specific fatigue life properties. The problem is complicated by the different properties of each of sandwich components. The PCHSPs tests are always tests of the structural element. Therefore, the complications re- indexed on: http://www.scopus.com sulting from the demands of adhesive bonding technology are increasing due to the known factors affecting the number of the achieved cycles, ie. stress values, structure of the individual components, geometric shape and dimensions. This also explains non-existent standard for the PCHSP ´s fatigue test. The fatigue testing methodology have to always include a statistical approach for the evaluation of the test results and with respect to the loading and conducted cycles itself we differ between low and high-cycle fatigue [12-16]. The statistical evaluation of the PCHSPs fatigue tests results is in a graphical representation using the classic S-N (Wöhler) curve and it determinines the reliability of the estimates of statistical variables. As a result, median of lifetime, the shortest life and the lower limit of fatigue life were investiquded in this work. During fatigue testing, it is advisable to monitor the formation and propagation of the sample´s damage by infrared thermography. This non-destructive testing method is very well suited in CM and PCHSP testing and it has been validated in other experiments, eg. in [17]. Experiment 2.1 Materials For the static and fatigue tests, the same samples were manufactured. Three prepreg layers in each side of facings were used for the fabrication of the experimental samples. Prepreg from company G. Angeli was used, having trademark: IMP503Z / VV 192 T. The glass fiber fabric had twill weave with density of 202 g/m2. The resin content in the prepreg was 33 vol. %. Aluminum honeycomb from EURO-COMPOSITES, trademark: ECM 6.4-60, was used as the core with thickness of 8 mm. The aluminum alloy was Alu-Alloy 3003 (AlMnCu) coated with zirconia. Density of this honeycomb was 60 kg/m3 having cell size of 6.4 mm. The sandwich sample cut by water jet from manufactured panel is shown in Fig. 1. 727 October 2018, Vol. 18, No. 5 MANUFACTURING TECHNOLOGY ISSN 1213–2489 Fig. 1 Sample of Polymer composite honeycomb sandwich panels (PCHSPs) maximum stress was set to the specified levels by changing the configuration of the test device. The time until the complete sample failure was measured. The results of the fatigue tests were statistically evaluated at each level separately. The tests results sets were assumed to have the number of cycles logarithms according to the normal distribution. For each level, the arithmetic mean of the number of measured cycles ̅ ,the median of the measured cycles , the standard deviation of the measured cycles s and the variation coefficient Vx (Tab. 3) were calculated. In order to calculate other statistical characteristics, the sample mean, as the best estimation of the mean value of the base set E, was calculated according to equation (2): The connection of the prepreg with the honeycomb was achieved by compression molding technology, which was carried out at 125° C (with a hour start and subsequent cooling). Prepared sandwich samples dimensions were following; l = 200 mm, b = 43 mm and h = 9 mm. Used dimensions was inaccordance with ČSN EN 2374 standard [18]. [-] (2) Where: ̂ …The sample mean [-], Xi…The i-th value of the observed test file (in log10) [-], n…The number of data sets [-]. The "^" means that it is an estimate based on the test file. The sample standard deviation was calculated according to Equation (3): ∑ ∑ 2.2 Experimental apparatus, equipment and methods The three-point bending static test was performed in accordance to ČSN EN 2562 and ČSN EN ISO 14125 [19, 20] on Universal testing machine Zwick 1456. Testing temperature was 23 °C. Test speed was set to 5 mm/min with support span equal to 178 mm. The test is based on the fact that the sample is bent at a constant speed to its fracture. During the test, the force at failure of FB,i and deflection of fB,i were measured (Tab. 1). A Equation (1) was used to calculate the stress in the sample at damage and for each fatigue loading level: ∙ ∙ ∙ ∙ [MPa] (1) Where: σfb…Maximal stress of the sample at fracture point [MPa], FB…Size of the force [N] applied to the sample at its fracture in N-cycle, L…Distance [mm] between the supports of the test instrument (178 mm) b…Sample width [mm] (43 mm), h…The height of the sample (9 mm). The fatigue tests were carried out on a proprietary test device. This device has a classic, adjustable crank mechanism with a piston rod driven by gears with an electromotor with variable speed. The device is not capable of measuring load force Fmax, i. However, at known engine speeds and gear ratios, the number of the measured cycles can be achieved by the time measuring. The fatigue test was performed at three stress levels. The levels were determined as a percentage of the force obtained from static three-point bend test (FB). According to Tab. 2, it was 75%, 55% and 45% of the arithmetic mean FB. Despite the impossibility of controlling the load force, a soft loading was used. The load waveform for each level was cyclic, sinusoidal, and passing (lower stress σmin = 0, coefficient of cycle asymmetry R = 0). The 728 [-] (3) Where: σ…Te sample standard deviation [-], Xi…The i-th value of the observed test file (in log10) [-], ̂ …The sample mean [-], n…The number of data sets [-] (n = 5). Median of lifetime was calculated according to Equation (4): ; $% ";# ; &" [-] (4) Where: ' (;) *;+ ...The median of lifetime in the number of cycles at the probability by P (predictive reliability) [%], 1-α…The confidence level of reliability, and v is the number of degrees of freedom [-] (n - 1 = 4). The estimate of cycles number of the shortest lifetime that survives 95% of all samples was calculated according to Equation (5): $ $ ,-./∗ [-] (5) Where: '1 ...The shortest lifetime in numbero of cycle [-], ̂ …The sample mean [-], σ…The sample standard deviation [-], and the constant of 1.645 was determined from the tables in [1] to survive 95% of all samples. The lower limit of fatigue life for x-th % probability of failure at a confidence level x%, where the unilateral tolerance limit of the normal distribution k(P;1-α;v) was calculated (Equation (6)). % ; " 23 , ",# ∗ [-] (6) Where: 4 (;) * …The lower limit of fatigue life in the number of cycles [-], indexed on: http://www.scopus.com October 2018, Vol. 18, No. 5 ̂ …The sample mean [-], 5 (,) MANUFACTURING TECHNOLOGY *,+ is the unilateral to- lerance limit of the normal distribution, and σ is the sample standard deviation. By combining the calculated values, the Wöhler curve (S-N curve) was obtained, representing a 95% survival limit in this particular experiment. A regression nonlinear least squares method was used to compensate for the S-N curve. ISSN 1213–2489 Results and Discussion 3.1 Static test - three-point bending The results of the static three-point bending test of the five samples are shown in Tab. 1. The standard deviation complies with Sillen's rule (the estimated parameter should be greater than three times its standard deviation value). Tab. 1 Static test results in three-point bending Sample No.: 1 Strength at failure FB,i [N] Bend at failure fB,i [mm] Stress at failure σfB [MPa] 2 3 4 712 946 843 887 4.6 6.5 5.7 6.2 Calculated accord. to equation (1): 3.2 Fatigue test According to the methodology which is referred in paragraph 2.3.2, and by using the Equation (1) the three load levels σmax,i = 50, 37 and 30 MPa, were determined. These Tab. 2 Determination of load levels Level No. % from FB,i [%] Force Fmax,i [N] 75 668 1 55 490 2 45 400 3 1068 7.3 891 6.1 67.5 Standard deviation s [-] 117.2 0.9 levels are given in Tab. 2 and 3. According to the description of the test equipment in paragraph 2.2.2, the number of (measured) Ni cycles and the calculated statistical characteristics (Tab. 3) were specified. Bend fmax,i [mm] 4.6 3.4 2.1 Tab. 3 shows that for each stress level the difference between the arithmetic mean of the measured cycles number x ̅, the median of the measured cycles x ̃, and the median of lifetime ' )1 is insignificant. This is evidence of correctly performed fatigue tests including samples fabrication. The median of lifetime ' )1 means that in further tests at the same stress level, about half of the samples will have a lifetime of less than 181, 30509, and 1157910 cycles. In order to assess the reliability of the structure, the shortest lifetime of '1 (106, 25704, and 829688 5 Arithmetic 6 [-] mean % Maximum stress σmax,i [MPa] 50 37 30 Stress amplitude σa,i [MPa] 25.0 18.5 15.0 cycles) is most important, surviving 95% of all samples. In fact, either the mean value or the scattering reliably is not known, because they were determined from five samples at each level. The coefficient of 1.645 in Equation (5) can be replaced by another coefficient for the unilateral tolerance limit k(P;1-α;v) of Equation (6) and determining the lower limit of fatigue life 4 (10) (45, 19702, and 494196 cycles). It is quite obvious that the lower limit of the fatigue life 4 (10) is considerably lower than the shortest lifetime '1 . This difference shows that the fatigue test was performed with a small number of samples. Tab. 2 Fatigue test results and statistical characteristics Number of measured cycles Ni [-] 6 [-] Arithmetic mean of the number of measured cycles % 7 [-] Median of measured cycles % Standard deviation of measured cycles s [-] Variation coefficient Vx [%] Median of lifetime (10) [-] Shortest lifetime 0 [-] Lower limit of fatigue life %(10) [-] indexed on: http://www.scopus.com Level No.1 σmax,1 = 50 MPa 158 197 283 116 189 189 189 61,6 32.7 181 106 46 Level No. 2 σmax,2 = 37 MPa 32712 28274 31082 26708 34429 30642 31082 3159 10.3 30509 25704 19702 Level No.3 σmax,3 = 30 MPa 1055090 1418403 1453173 1036366 923536 1177314 1055090 241573 20.5 1157910 829688 494196 729 October 2018, Vol. 18, No. 5 MANUFACTURING TECHNOLOGY 3.3 S-N (Wöhler) curve The Wöhler curve (S-N curve) was obtained by combining the calculated median lifetime ' )1 and the values of the individual stress levels, representing a 95% survival limit in this particular experiment. Fig. 2 shows the graphical representation of the Wöhler curve. For the ISSN 1213–2489 clarity of the chart, there are no other statistical characteristics mentioned (eg. lower limit). For the regression analysis, the Solver from MS Office-Excel was used. The confidence value R2 = 0.9946 is very close to 1. This confirms the appropriately chosen regression method (regression nonlinear least squares method). Uniform scales (x and y axes) were used intentionally. Fig. 2 S-N (Wöhler) curve Conclusion In the research, static bending properties and fatigue life of prepared honeycomb core sandwich samples have been investigated. Conducted tests and used statistical evaluation provided interesting results that are applicable PCHSP evaluation and design. From obtained Wöhler curve shape, it is observed that the stress level σmax, 3 = 30 MPa is very close to the fatigue limit σc, where the sample would theoretically withstand an infinite number of cycles. All kinds of means of transport are designed for a given lifetime. This article describes the method that can be used to determine the basic lifetime characteristics of PCHSP´s. The knowledge of these characteristics is necessary in order the to be designed not only for static strength but also for the required fatigue life. Acknowledgement The authors gratefully acknowledge the financial support of this research by the internal grant of Tomas Bata University in Zlín No. Zlín No. IGA/FT/2018/004 funded from the resources of specific university research. 730 References ČSN 42 0368. Fatigue testing of metals. Statistical evaluation of fatigue test results of metals. Praha: ÚNMZ. 1973. ČSN ISO 12107. Metallic materials. Fatigue testing. Statistical planning and analysis of data. Praha: ÚNMZ 2013. GOST 33845-2016 (ISO 13003:2003) Polymer composites. Test method for fatigue properties under cyclic loading conditions. Moscow: EASC. 2017. MIL-HDBK-23A Structural Sandwich Composites. Washington: USA, Department of Defense. 1974. BITZER, T. Honeycomb Technology Materials, Design, Manufacturing, Applications and Testing. Dordrecht: Springer Netherlands, 1997, 233 s. ISBN 978-940-1158-565 VASSILOPOULOS, A. P. Fatigue life prediction of composites and composite structures. Oxford: indexed on: http://www.scopus.com October 2018, Vol. 18, No. 5 MANUFACTURING TECHNOLOGY ISSN 1213–2489 Woodhead Publishing, 2010, 552 s. ISBN 978-184569-525-5 Technology, Vol. 16, Issue 2, pp. 375-380, ISSN 1213-2489. BELOUETTAR, S., ABBADI, A. AZARI, Z., BELOUETTAR, R. FRERES, P. (2009) Experimental investigation of static and fatigue behaviour of composites honeycomb materials using four point bending tests. Composite Structures. Vol. 87, Issue 3, pp. 265-273. ISSN 0263-8223 ŠLEGER, V., MÜLLER, M. (2016) Low-Cyclic Fatigue of Adhesive Bonds. Manufacturing Technology, Vol. 16, Issue 5, pp. 1151-1157, ISSN 1213-2489. ABBADI, A., TIXIER, C., GILGERT, J., AZARI, Z. (2015) Experimental study on the fatigue behaviour of honeycomb sandwich panels with artificial defects. Composite Structures, Vol. 120, pp. 394-405. ISSN 0263-8223 BOUKHAROUBA, W., BEZAZI, A., SCARPA, F. (2014) Identification and prediction of cyclic fatigue behaviour in sandwich panels. Measurement. 2014, Vol. 53, pp. 161-170. ISSN 02632241 WAHL, L., MAAS, S., WALDMANN, D., ZÜRBES, A., FRÈRES, P. (2013) Fatigue in the core of aluminum honeycomb panels: Lifetime prediction compared with fatigue tests. International Journal of Damage Mechanics. Vol. 23, Issue 5, pp. 661-683. ISSN 1056-7895. Some fatigue characteristics of sandwich material with honeycomb core. (1972) Praha: VZLÚ KUCHARIKOVÁ, L., TILLOVÁ, E., UHRÍČIK, M., BELAN, J., ŠVECOVÁ, I. (2017) High-cycles Fatigue of Different Casted Secondary Aluminium Alloy. Manufacturing Technology, Vol. 17, Issue 5, pp. 756-761, ISSN 1213-2489. NOVÝ, F., KOPAS, P., BOKŮVKA, O., SAVIN, A. (2016) Reparation by Hard Facing of the Damaged Secondary Stone Crushers. Manufacturing UHRÍČIK, M., ORAVCOVÁ, M., PALČEK, P., CHALUPOVÁ, M. (2016) The Stress Detection and the Fatigue Lifetime of Stainless Steel during Three-Point Bending Cyclic Loading. Manufacturing Technology, Vol. 16, Issue 5, pp. 11791182, ISSN 1213-2489. ZAVRTÁLEK, J., MÜLLER, M. (2016) Low-cyclic Fatigue Test of Adhesive Bond Reinforced with Biodegradable Fabrics. Manufacturing Technology, Vol. 16, Issue 5, pp. 1205-1211, ISSN 1213-2489. VAVILOV, V.P., BUDADIN, O.N., KULKOV, A.A. (2014) Infrared thermographic evaluation of large composite grid parts subjected to axial loading. Polymer Testing. Vol. 41, pp. 55-62. ISSN 0142-9418. ČSN EN 2374. Aerospace series. Glass fibre reinforced mouldings and sandwich coposites. Production of test panels. Praha: ÚNMZ. 1996. ČSN EN 2562 Aerospace series. Carbon fibre reinforced plastics. Unidirectional laminates. Flexural test paralle to the fibre direction. Praha: ÚNMZ. 1999. ČSN EN ISO 14125 Fibre-reinforced plastic composites. Determination of flexural properties. Praha: ÚNMZ. 1999. 10.21062/ujep/167.2018/a/1213-2489/MT/18/5/727 Copyright © 2018. Published by Manufacturing Technology. All rights reserved. indexed on: http://www.scopus.com 731